Tests of One-Way
With Unbonded Tendons
Ned H. Burns
Professor of Civil Engineering
The University of Texas at Austin
Finley A. Charney*
Walter P. Moore & Associates, Inc.
Wendell R. Vines*
The provisions in the ACI BuildingCode (ACI 318-77)1 for pre-
stressed concrete recognize a differ-
ence in the amount of mild steel re-
quired for ultimate strength and crack
control between bonded and un-
bonded members. However, the ACI
Code equations are based mainly on
experience with and tests on beams
with relatively low span/depth ratios
compared to those common with
Previous research efforts concern-
ing members with unbonded tendons
and various span/depth ratios have
shown that the ACI• Code expressions
for steel stress at ultimate may be un-
conservative for members such as
slabs with span/depth ratios as high
as 40 or more, 2' 3 while reinforcement
required for crack control may be on
the conservative side.
`Formerly Research Assistants, The University of
Texas at Austin.
In order to obtain a better under-
standing of partially prestressed con-
crete slabs with unbonded tendons, a
test program was carried out at The
University of Texas at Austin during
which the strength and behavior of
two half-scale models of prototype
structures were experimentally
evaluated 4 '5 Of major concern was
the comparison of observed behavior
with that predicted following the
provisions of ACI 318-77.
The specific objectives of the test
program were to:
1. Examine the load-deflection re-
sponse of the slabs before and
after initial cracking with par-
ticular attention to the effects of
cracking on the observed stiff-
ness of the two slabs.
2. Observe the control and dis-
tribution of cracking provided by
different amounts of bonded
3. Determine experimentally the
ultimate strength of the speci-
mens as well as measure the in-
crease in tendon stresses as fail-
ure loads were approached.
4. Compare the test results with the
provisions contained in ACI
Prestressed concrete elements are
normally proportioned on the basis of
some limiting stress in the concrete at
service load, and then checked for ul-
timate strength. Depending on the
magnitude of the tensile stress in the
concrete, the service load deflections
may or may not be elastic.
Under normal circumstances, the
limiting tensile stress is 6 fI
(0.50 f,') and the concrete remains
uncracked throughout the service load
range. Section 18.4.2 of the ACI Code,
however, allows tensile stresses as
PCI JOURNAUSeptember-October 1978 67
Table 1. Design parameters of prototype structures for
Slabs A and B.
Parameter Prototype for
Span 20 ft. 20 ft.
Slab thickness 5.5 in. 5.5 in.
Design live load 50 psf 50 psf
Allowable tension in
concrete at service
load 6/ 91/f^
f/ 4000 psi 4000 psi
240 ksi 240 ksi
213 ksi 213 ksi
P/A stress 185 psi 140 psi
Initial tendon stress 140 ksi 140 ksi
reinforcement 0.120 0.098
Percent bonded 0.12 < 0.20 0.23 > 0.20
reinforcement required by required by
ACI Code ACI Code
*Two adjacent spans loaded with live load and dead load on all spans.
Note: 1 psi = 6.9 kN/mz ; 1 ksi = 6.89 MPa; 1 ft = 0.305m; 1 in. = 25.4 mm; 1 lb = 4.45 N.
high as 12[ (1.00 f, ), so long as
careful deflection computations are
made to insure satisfactory perfor-
mance. With service load stresses of
12 J7,' (1.00 f,) the concrete would
certainly be cracked (fr = 7.5 fJ or
0.62 f,') and inelastic action would
be evident in the working load range.
In addition to the requirements for
maximum tensile stresses in the con-
crete, ACI 318-77 states a minimum
requirement for bonded reinforce-
ment when unbonded tendons are
A, = 0.004A [ACI Eq. (18-5)]
A, = minimum bonded steel, sq in.
A = area of that part of the cross
section between the flexural
tension face and the center of
gravity of cross section, sq in.
Eq. (18-5) requires that A, for a solid
slab equal to 0.2 percent of the cross-
sectional area be supplied as bonded
reinforcement, and a primary question
to be addressed by these tests is
whether this amount of A, is realistic
as a minimum requirement.
Two slabs were experimentally
evaluated incorporating characteristics
to test the adequacy of the ACI Code
design requirements. The main vari-
ables in the two specimens were the
allowable tensile stress in the con-
crete at service load and the amount of
bonded reinforcement. In Slab A, the
tensile stresses were limited to 6 JJ
(0.50 f) and in Slab B, the design
tensile stresses under service load
were 9J7 (0.75/7). ). In both cases
the bonded reinforcement provided
was that required for strength, even if
that amount were less than that
A 2 B 3 C 4
2.25=l •° • Section A-A•
55" I 6fc at Sec. 2-2 with service load
0 1/4° 0 unbonded tendon
2.25" Section 2-2 • No.2 deformed bar
2 .2 511111 ° ° I Section B-B
Note: 1 ft = 0.305 m; 1 in. = 25.4 mm.
Fig. 1 a. Plan and section of Slab A (ideal model).
2 B 3 C
2.25" C ..° • .° ..° • Section A-A
L 55 I 9/i at Sec. 2-2 with service load
0 1/4" 0 unbonded tendon
2.25° EllIll * *° * .° . 0° 0 I Section 2-2 • No. 2 deformed bar
2.25" IlII ° • ° • ° Section B-B
Note: 1 ft = 0.305 m; 1 in. = 25.4 mm.
Fig. 1b. Plan and section of Slab B (ideal model).
specified under Section 18.9 of the
ACI Code. For Slab A (prototype and
model) the bonded reinforcement was
0.12 percent of cross-sectional area
which is less than the 0.20 percent re-
quired by the ACI Code.
The physical dimensions of the
prototype slabs were the same for
both specimens; three equal spans of
20 ft (6 m) each, and a thickness of 5.5
in. (140 mm).
Table 1 lists the design parameters
for the prototype structures. Test slabs
A and B were half-scale models from
Figs. la and lb show a plan and
section views for the two slab speci-
PCI JOURNAL/September-October 1978 69
With the design conditions known,
the two one-half scale model struc-
tures (Slab A and Slab B) were pro-
portioned accordingly. By matching the
PIA stresses in the prototype, the
width of the specimens was set as 55
in. (1400 mm). Using this width, scal-
ing all other dimensions down to
one-half, and replacing the weight of
concrete lost due to scaling, the mod-
els would be stressed exactly as would
the prototype under similar loading
The prototype slabs and half-scale
models were designed for a 28-day
compressive concrete strength of 4000
psi (27.58 MPa). The observed
strength for the models was higher
with a measured average cylinder
strength of 4700 psi (32.41 MPa) for
Slab A and 5150 psi (35.51 MPa) for
Slab B. The unbonded tendons were
Y4 in. (6.3 mm) diameter single wire
with a measured ultimate strength of
240 ksi (1655 MPa). The tendons were
coated with mastic and wrapped in
reinforced waterproof paper to pre-
vent bond to the concrete. The
bonded reinforcement was deformed
bar of 6 mm diameter (#2 bar) with a
yield stress of 65 ksi (448 MPa).
The specimens were cast in place
over pedestals which provided line
support across the width of the slab.
Refer to Fig. 2 for the nomenclature
used in this paper for identifying sup-
ports and spans.
1 A 2 B 3 C 4
Fig. 2. Identifying nomenclature.
Both slabs were extensively in-
strumented. Stresses in tendons and
bonded reinforcement were moni-
tored using strain gages. Midspan and
quarter span deflections were mea-
sured electronically and checked
manually with dial gages. Load cells
monitored interior support reactions,
applied, loads, and force in the un-
x in" I Load Pates Q
Fig. 3. Plan and elevation of loading system used in tests.
Note: 1 ft = 0.305 m; 1 in. = 25.4 mm.
1 A 2 8 3 C
Fig. 4a. Load patterns for Slab A. Note: 1 psf = 47.9 Pa.
Note: Loads Shown in units psf (Applied Loads) 115
69 psf Dead
Load (Typ. I A 2 8 3 C 4All Tests)
27.5 159 27.5
=0.4 D.L.I = 0.4 D.L.
Fig. 4b. Load patterns for Slab B. Note: 1 psf = 47.9 Pa.,
Pattern loadings designed to pro-
duce maximum stress at each critical
section were imposed on the slabs.
Fig. 3 illustrates the whiffle tree
mechanism used to simulate a uniform
load on the slabs. The specimens
were tested through three load ranges:
elastic, inelastic (cracked), and ulti-
Figs. 4a and 4b show the patterns of
loadings used in the tests. Load levels
PCI JOURNAL/September-October 1978 71